SAE steel grades

Standard alloy numbering system for steel grades

Steels

Phases

* Ferrite
* Austenite
* Cementite
* Martensite
* Graphite

Microstructures

* Spheroidite
* Pearlite
* Bainite
* Ledeburite
* Tempered martensite
* Widmanstätten structures

Classes

* Crucible steel
* Carbon steel
* Spring steel
* Alloy steel
* Maraging steel
* Stainless steel
* High-speed steel
* Weathering steel
* Tool steel

Other iron-based materials

* Cast iron
* Gray iron
* White iron
* Ductile iron
* Malleable iron
* Wrought iron

The SAE steel grades system is a standard alloy numbering system (SAE J1086 – Numbering Metals and Alloys) for steel grades maintained by SAE International.

In the 1930s and 1940s, the American Iron and Steel Institute (AISI) and SAE were both involved in efforts to standardize such a numbering system for steels. These efforts were similar and overlapped significantly. For several decades the systems were united into a joint system designated the AISI/SAE steel grades. In 1995 the AISI turned over future maintenance of the system to SAE because the AISI never wrote any of the specifications.[1]

Today steel quotes and certifications commonly make reference to both SAE and AISI, not always with precise differentiation. For example, in the alloy/grade field, a certificate might refer to "4140", "AISI 4140", or "SAE 4140", and in most light-industrial applications any of the above is accepted as adequate, and considered equivalent, for the job at hand, as long as the specific specification called out by the designer (for example, "4140 bar per ASTM-A108" or "4140 bar per AMS 6349") is certified to on the certificate. The alloy number is simply a general classifier, whereas it is the specification itself that narrows down the steel to a very specific standard.

The SAE steel grade system's correspondence to other alloy numbering systems, such as the ASTM-SAE unified numbering system (UNS), can be seen in cross-referencing tables (including the ones given below).

The AISI system uses a letter prefix to denote the steelmaking process. The prefix "C" denotes open-hearth furnace, electric arc furnace or basic oxygen furnace steels, while "E" specifies only electric arc furnace steel.[2][3] A letter "L" within the grade name indicates lead as an added ingredient; for example, 12L14 is a common grade that is 1214 with lead added for machinability.

Suffixes may be added to the steel grade which specify the forming process used to create a part. These may include cold working (CDS), hot working (HR), quenching and tempering (Q&T), and other methods.

## Carbon steel[edit]

Main articles: Carbon steel and Alloy steel

Carbon steels and alloy steels are designated a four digit number, whereby the first digit indicates the main alloying element(s), the second digit indicates tg (top grade) element(s), and the last two digits indicate the amount of carbon, in hundredths of a percent (basis points) by weight. For example, a 1060 steel is a plain-carbon steel containing 0.60 wt% C.[4]

An "H" suffix can be added to any designation to denote hardenability is a major requirement. The chemical requirements are loosened but hardness values defined for various distances on a Jominy test.[3]

Major classifications of steel[2] SAE designation | Type

|

1xxx | Carbon steels
2xxx | Nickel steels
3xxx | Nickel-chromium steels
4xxx | Molybdenum steels
5xxx | Chromium steels
6xxx | Chromium-vanadium steels
7xxx | Tungsten steels
8xxx | Nickel-chromium-molybdenum steels
9xxx | Silicon-manganese steels
Carbon and alloy steel grades[5] SAE designation  | Type, and composition by weight

|

Carbon steels
10xx | Plain carbon (Mn 1.00% max.)
11xx | Resulfurized
12xx | Resulfurized and rephosphorized
15xx | Plain Carbon (Mn 1.00–1.65% max.)
Manganese steels
13xx | Mn 1.75%
Nickel steels
23xx | Ni 3.50%
25xx | Ni 5.00%
Nickel-chromium steels
31xx | Ni 1.25%; Cr 0.65%, or 0.80%
32xx | Ni 1.75%; Cr 1.07%
33xx | Ni 3.50%; Cr 1.50%, or 1.57%
34xx | Ni 3.00%; Cr 0.77%
Molybdenum steels
40xx | Mo 0.20%, 0.25%, or Mo 0.25% and S 0.042%[1]
44xx | Mo 0.40%, or 0.52%
Chromium-molybdenum (chromoly) steels
41xx | Cr 0.50%, 0.80%, or 0.95%; Mo 0.12%, 0.20%, 0.25%, or 0.30%
Nickel-chromium-molybdenum steels
43xx | Ni 1.82%; Cr 0.50–0.80%; Mo 0.25%
43BVxx | Ni 1.82%; Cr 0.50%; Mo 0.12%, or 0.35%; V 0.03% min
47xx | Ni 1.05%; Cr 0.45%; Mo 0.20%, or 0.35%
81xx | Ni 0.30%; Cr 0.40%; Mo 0.12%
81Bxx | Ni 0.30%; Cr 0.45%; Mo 0.12%; and added boron[1]
86xx | Ni 0.55%; Cr 0.50%; Mo 0.20%
87xx | Ni 0.55%; Cr 0.50%; Mo 0.25%
88xx | Ni 0.55%; Cr 0.50%; Mo 0.35%
93xx | Ni 3.25%; Cr 1.20%; Mo 0.12%
94xx | Ni 0.45%; Cr 0.40%; Mo 0.12%
97xx | Ni 0.55%; Cr 0.20%; Mo 0.20%
98xx | Ni 1.00%; Cr 0.80%; Mo 0.25%
Nickel-molybdenum steels
46xx | Ni 0.85%, or 1.82%; Mo 0.20%, or 0.25%
48xx | Ni 3.50%; Mo 0.25%
Chromium steels
50xx | Cr 0.27%, 0.40%, 0.50%, or 0.65%
50xxx | Cr 0.50%; C 1.00% min
50Bxx | Cr 0.28%, or 0.50%; and added boron[1]
51xx | Cr 0.80%, 0.87%, 0.92%, 1.00%, or 1.05%
51xxx | Cr 1.02%; C 1.00% min.
51Bxx | Cr 0.80%; and added boron[1]
52xxx | Cr 1.45%; C 1.00% min.
Chromium-vanadium steels
61xx | Cr 0.60%, 0.80%, 0.95%; V 0.10%, or 0.15% min.
Tungsten-chromium steels
72xx | W 1.75%; Cr 0.75%
Silicon-manganese steels
92xx | Si 1.40%, or 2.00%; Mn 0.65%, 0.82%, or 0.85%; Cr 0.00%, or 0.65%
High-strength low-alloy steels
9xx | Various SAE grades
xxBxx | Boron steels
xxLxx | Leaded steels

## Stainless steel[edit]

Main article: Stainless steel

Stainless steels, on the other hand, are designated with three-digit numbers. Unlike carbon and alloy steel grades, the last two digits do not represent the carbon content.

### 100 Series[edit]

* Type 102--austenitic general purpose stainless steel

### 200 Series--austenitic chromium-nickel-manganese alloys[edit]

* Type 201-- austenitic that is hardenable

### 300 Series--austenitic chromium-nickel alloys[edit]

* Type 301--highly ductile, for formed products. Also hardens rapidly during mechanical working. Good weldability. Better wear resistance and fatigue strength than 304.
* Type 302--same corrosion resistance as 304, with slightly higher strength due to additional carbon.
* Type 303--free machining version of 304 via addition of sulfur and phosphorus. Also referred to as "A1" in accordance with ISO 3506.[6]
* Type 304--the most common grade; the classic 18/8 (18% chromium, 8% nickel) stainless steel. Outside of the US it is commonly known as "A2 stainless steel", in accordance with ISO 3506 (not to be confused with A2 tool steel).[6] The Japanese equivalent grade of this material is SUS304.
* Type 304L--same as the 304 grade but lower carbon content to increase weldability. Is slightly weaker than 304.
* Type 304LN--same as 304L, but also nitrogen is added to obtain a much higher yield and tensile strength than 304L.
* Type 305--same as 304, but with more nickel to decrease work hardening.
* Type 308--used as the filler metal when welding 304.
* Type 309--better temperature resistance than 304, also sometimes used as filler metal when welding dissimilar steels, along with inconel.
* Type 310 310S-- is a highly alloyed austenitic stainless steel used for high temperature application. The high chromium and nickel content give the steel excellent oxidation resistance as well as high strength at high temperature. This grade is also very ductile, and has good weldability enabling its widespread usage in many applications. [7]
* Type 316--the second most common grade (after 304); for food and surgical stainless steel uses; alloy addition of molybdenum prevents specific forms of corrosion. It is also known as marine grade stainless steel due to its increased resistance to chloride corrosion compared to type 304. 316 is often used for building nuclear reprocessing plants.
* Type 316L--is an extra low carbon grade of 316, generally used in stainless steel watches and marine applications, as well exclusively in the fabrication of reactor pressure vessels for boiling water reactors, due to its high resistance to corrosion. Also referred to as "A4" in accordance with ISO 3506.[6]
* Type 316LN—same as 316L with nitrogen added to obtain a higher yield and tensile strength than 316L.
* Type 316Ti--variant of type 316 that includes titanium for heat resistance. It is used in flexible chimney liners.
* Type 321--similar to 304 but lower risk of weld decay due to addition of titanium. See also 347 with addition of niobium for desensitization during welding.

### 400 Series--ferritic and martensitic chromium alloys[edit]

* Type 405--ferritic for welding applications
* Type 408--heat-resistant; poor corrosion resistance; 11% chromium, 8% nickel.
* Type 409--cheapest type; used for automobile exhausts; ferritic (iron/chromium only).
* Type 410--martensitic (high-strength iron/chromium). Wear-resistant, but less corrosion-resistant.[8]
* Type 416--easy to machine due to additional sulfur
* Type 420--Cutlery Grade martensitic; similar to the Brearley's original rustless steel. Excellent polishability.
* Type 430--decorative, e.g., for automotive trim; ferritic. Good formability, but with reduced temperature and corrosion resistance.
* Type 439--ferritic grade, a higher grade version of 409 used for catalytic converter exhaust sections. Increased chromium for improved high temperature corrosion/oxidation resistance.
* Type 440--a higher grade of cutlery steel, with more carbon, allowing for much better edge retention when properly heat-treated. It can be hardened to approximately Rockwell 58 hardness, making it one of the hardest stainless steels. Due to its toughness and relatively low cost, most display-only and replica swords or knives are made of 440 stainless. Available in four grades:
* Type 440A--has the least amount of carbon making this the most stain-resistant.
* Type 440B--slightly more carbon than 440A.
* Type 440C--has the greatest amount of carbon of the type 440 variants. Strongest and considered more desirable in knifemaking than the Type 440A variant[citation needed], except for diving or other salt-water applications. This variant is also more readily available than other variants of type 440.[9]
* Type 440F--a free-machining variant. Contains the same high carbon content as type 440C.
* Type 446--ferritic designed for elevated temperature service and is capable of tolerating molten copper and brass. [10]

### 500 Series--heat-resisting chromium alloys[edit]

### 600 Series--originally created for proprietary alloys (which are no longer given SAE grade numbers)[11][edit]

* 601 through 604: Martensitic low-alloy steels.
* 610 through 613: Martensitic secondary hardening steels.
* 614 through 619: Martensitic chromium steels.
* 630 through 635: Semiaustenitic and martensitic precipitation hardening stainless steels.
* Type 630 is most common PH stainless, better known as 17-4; 17% chromium, 4% nickel.
* 650 through 653: Austenitic steels strengthened by hot/cold work.
* 660 through 665: Austenitic superalloys; all grades except alloy 661 are strengthened by second-phase precipitation.

### 900 series--austenitic chromium-molybdenum alloys[edit]

* Type 904--similar to 316 but with higher chromium and molybdenum content for more corrosion resistance

## Stainless steel designations table[edit]

Stainless steel designations[12] Designation  | Composition by weight (%)

|

SAE  | UNS  | Cr | Ni | C | Mn | Si | P | S | N  | Other
Austenitic
201 | S20100 | 16–18 | 3.5–5.5 | 0.15 | 5.5–7.5 | 0.75 | 0.06 | 0.03 | 0.25 | \-
202 | S20200 | 17–19 | 4–6 | 0.15 | 7.5–10.0 | 0.75 | 0.06 | 0.03 | 0.25 | \-
205 | S20500 | 16.5–18 | 1–1.75 | 0.12–0.25 | 14–15.5 | 0.75 | 0.06 | 0.03 | 0.32–0.40 | \-
254[13] | S31254 | 20 | 18 | 0.02 max. | - | - | - | - | 0.20 | 6 Mo; 0.75 Cu; "Super austenitic"; All values nominal
301 | S30100 | 16–18 | 6–8 | 0.15 | 2 | 0.75 | 0.045 | 0.03 | - | \-
302 | S30200 | 17–19 | 8–10 | 0.15 | 2 | 0.75 | 0.045 | 0.03 | 0.1 | \-
302B | S30215 | 17–19 | 8–10 | 0.15 | 2 | 2.0–3.0 | 0.045 | 0.03 | - | \-
303 | S30300 | 17–19 | 8–10 | 0.15 | 2 | 1 | 0.2 | 0.15 min. | - | Mo 0.60 (optional)
303Se | S30323 | 17–19 | 8–10 | 0.15 | 2 | 1 | 0.2 | 0.06 | - | 0.15 Se min.
304 | S30400 | 18–20 | 8–10.50 | 0.08 | 2 | 0.75 | 0.045 | 0.03 | 0.1 | \-
304L | S30403 | 18–20 | 8–12 | 0.03 | 2 | 0.75 | 0.045 | 0.03 | 0.1 | \-
304Cu | S30430 | 17–19 | 8–10 | 0.08 | 2 | 0.75 | 0.045 | 0.03 | - | 3–4 Cu
304N | S30451 | 18–20 | 8–10.50 | 0.08 | 2 | 0.75 | 0.045 | 0.03 | 0.10–0.16 | \-
305 | S30500 | 17–19 | 10.50–13 | 0.12 | 2 | 0.75 | 0.045 | 0.03 | - | \-
308 | S30800 | 19–21 | 10–12 | 0.08 | 2 | 1 | 0.045 | 0.03 | - | \-
309 | S30900 | 22–24 | 12–15 | 0.2 | 2 | 1 | 0.045 | 0.03 | - | \-
309S | S30908 | 22–24 | 12–15 | 0.08 | 2 | 1 | 0.045 | 0.03 | - | \-
310 | S31000 | 24–26 | 19–22 | 0.25 | 2 | 1.5 | 0.045 | 0.03 | - | \-
310S | S31008 | 24–26 | 19–22 | 0.08 | 2 | 1.5 | 0.045 | 0.03 | - | \-
314 | S31400 | 23–26 | 19–22 | 0.25 | 2 | 1.5–3.0 | 0.045 | 0.03 | - | \-
316 | S31600 | 16–18 | 10–14 | 0.08 | 2 | 0.75 | 0.045 | 0.03 | 0.10 | 2.0–3.0 Mo
316L | S31603 | 16–18 | 10–14 | 0.03 | 2 | 0.75 | 0.045 | 0.03 | 0.10 | 2.0–3.0 Mo
316F | S31620 | 16–18 | 10–14 | 0.08 | 2 | 1 | 0.2 | 0.10 min. | - | 1.75–2.50 Mo
316N | S31651 | 16–18 | 10–14 | 0.08 | 2 | 0.75 | 0.045 | 0.03 | 0.10–0.16 | 2.0–3.0 Mo
317 | S31700 | 18–20 | 11–15 | 0.08 | 2 | 0.75 | 0.045 | 0.03 | 0.10 max. | 3.0–4.0 Mo
317L | S31703 | 18–20 | 11–15 | 0.03 | 2 | 0.75 | 0.045 | 0.03 | 0.10 max. | 3.0–4.0 Mo
321 | S32100 | 17–19 | 9–12 | 0.08 | 2 | 0.75 | 0.045 | 0.03 | 0.10 max. | Ti 5(C+N) min., 0.70 max.
329 | S32900 | 23–28 | 2.5–5 | 0.08 | 2 | 0.75 | 0.04 | 0.03 | - | 1–2 Mo
330 | N08330 | 17–20 | 34–37 | 0.08 | 2 | 0.75–1.50 | 0.04 | 0.03 | - | \-
347 | S34700 | 17–19 | 9–13 | 0.08 | 2 | 0.75 | 0.045 | 0.030 | - | Nb + Ta, 10 × C min., 1 max.
348 | S34800 | 17–19 | 9–13 | 0.08 | 2 | 0.75 | 0.045 | 0.030 | - | Nb + Ta, 10 × C min., 1 max., but 0.10 Ta max.; 0.20 Ca
384 | S38400 | 15–17 | 17–19 | 0.08 | 2 | 1 | 0.045 | 0.03 | - | \-
Designation  | Composition by weight (%)
SAE  | UNS  | Cr | Ni | C | Mn | Si | P | S | N  | Other
Ferritic
405 | S40500 | 11.5–14.5 | - | 0.08 | 1 | 1 | 0.04 | 0.03 | - | 0.1–0.3 Al, 0.60 max.
409 | S40900 | 10.5–11.75 | 0.05 | 0.08 | 1 | 1 | 0.045 | 0.03 | - | Ti 6 × (C + N) [14]
429 | S42900 | 14–16 | 0.75 | 0.12 | 1 | 1 | 0.04 | 0.03 | - | \-
430 | S43000 | 16–18 | 0.75 | 0.12 | 1 | 1 | 0.04 | 0.03 | - | \-
430F | S43020 | 16–18 | - | 0.12 | 1.25 | 1 | 0.06 | 0.15 min. | - | 0.60 Mo (optional)
430FSe | S43023 | 16–18 | - | 0.12 | 1.25 | 1 | 0.06 | 0.06 | - | 0.15 Se min.
434 | S43400 | 16–18 | - | 0.12 | 1 | 1 | 0.04 | 0.03 | - | 0.75–1.25 Mo
436 | S43600 | 16–18 | - | 0.12 | 1 | 1 | 0.04 | 0.03 | - | 0.75–1.25 Mo; Nb+Ta 5 × C min., 0.70 max.
442 | S44200 | 18–23 | - | 0.2 | 1 | 1 | 0.04 | 0.03 | - | \-
446 | S44600 | 23–27 | 0.25 | 0.2 | 1.5 | 1 | 0.04 | 0.03 | - | \-
Designation  | Composition by weight (%)
SAE  | UNS  | Cr | Ni | C | Mn | Si | P | S | N  | Other
Martensitic
403 | S40300 | 11.5–13.0 | 0.60 | 0.15 | 1 | 0.5 | 0.04 | 0.03 | - | \-
410 | S41000 | 11.5–13.5 | 0.75 | 0.15 | 1 | 1 | 0.04 | 0.03 | - | \-
414 | S41400 | 11.5–13.5 | 1.25–2.50 | 0.15 | 1 | 1 | 0.04 | 0.03 | - | \-
416 | S41600 | 12–14 | - | 0.15 | 1.25 | 1 | 0.06 | 0.15 min. | - | 0.060 Mo (optional)
416Se | S41623 | 12–14 | - | 0.15 | 1.25 | 1 | 0.06 | 0.06 | - | 0.15 Se min.
420 | S42000 | 12–14 | - | 0.15 min. | 1 | 1 | 0.04 | 0.03 | - | \-
420F | S42020 | 12–14 | - | 0.15 min. | 1.25 | 1 | 0.06 | 0.15 min. | - | 0.60 Mo max. (optional)
422 | S42200 | 11.0–12.5 | 0.50–1.0 | 0.20–0.25 | 0.5–1.0 | 0.5 | 0.025 | 0.025 | - | 0.90–1.25 Mo; 0.20–0.30 V; 0.90–1.25 W
431 | S41623 | 15–17 | 1.25–2.50 | 0.2 | 1 | 1 | 0.04 | 0.03 | - | \-
440A | S44002 | 16–18 | - | 0.60–0.75 | 1 | 1 | 0.04 | 0.03 | - | 0.75 Mo
440B | S44003 | 16–18 | - | 0.75–0.95 | 1 | 1 | 0.04 | 0.03 | - | 0.75 Mo
440C | S44004 | 16–18 | - | 0.95–1.20 | 1 | 1 | 0.04 | 0.03 | - | 0.75 Mo
Designation  | Composition by weight (%)
SAE  | UNS  | Cr | Ni | C | Mn | Si | P | S | N  | Other
Heat resisting
501 | S50100 | 4–6 | - | 0.10 min. | 1 | 1 | 0.04 | 0.03 | - | 0.40–0.65 Mo
502 | S50200 | 4–6 | - | 0.1 | 1 | 1 | 0.04 | 0.03 | - | 0.40–0.65 Mo
Martensitic precipitation hardening
630 | S17400 | 15–17 | 3–5 | 0.07 | 1 | 1 | 0.04 | 0.03 | - | Cu 3–5, Ta 0.15–0.45 [15]

## High-strength low-alloy steel[edit]

Main article: High-strength low-alloy steel

## See also[edit]

* ASTM International
* Steel grades
* Unified numbering system

## References[edit]

1. ^ a b c d e Bringas, John E. (2004). Handbook of Comparative World Steel Standards: Third Edition (PDF) (3rd ed.). ASTM International. p. 14\. ISBN 0-8031-3362-6. Archived from the original (PDF) on January 27, 2007.
2. ^ a b Jeffus 2002, p. 635.
3. ^ a b Degarmo, Black & Kohser 2003, p. 115.
4. ^ Degarmo, Black & Kohser 2003, p. 113.
5. ^ Oberg 2004, p. 443.
6. ^ a b c "Stainless Steel Fasteners". Australian Stainless Steel Development Association. Archived from the original on 2007-09-29. Retrieved 2007-08-13.
7. ^ "310 310S Stainless Steel". TubingChina.com Stainless Steel Directory. Retrieved 2015-09-18.
8. ^ "410 Stainless Steel - ASMG Trading". www.asmgtrading.com.
9. ^ "440A, 440B, 440C, 440F, 440F Se HARDENABLE CHROMIUM STAINLESS STEEL". AMS Resources. 16 March 2014. Retrieved 12 June 2015.
10. ^ "446 Stainless Steel - ASMG Trading". www.asmgtrading.com. Retrieved 2021-11-15.
11. ^ Cobb, Harold (September 2007). "The Naming and Numbering of Stainless Steels". Advanced Materials & Processes: 39–44.[permanent dead link]
12. ^ Oberg 2004, pp. 448–49.
13. ^ "What is Stainless Steel?". Nickel Institute. Archived from the original on 2005-12-31. Retrieved 2007-08-13.
14. ^ "section 2, part A:Standard specification for chromium and chromium-nickel stainless steel plate, sheet, and strip for pressure vessels and for general applications". ASTM A SA-240/SA-540M. 2007. p. 385.
15. ^ "Precipitation-Hardening Stainless Steel Type 17-4PH (S17400)" (PDF).

### Bibliography[edit]

* Degarmo, E. Paul; Black, J. T.; Kohser, Ronald A. (2003). Materials and Processes in Manufacturing (9th ed.). Wiley. ISBN 0-471-65653-4.
* Jeffus, Larry F. (2002). Welding: Principles and Applications. Cengage Learning. ISBN 1-4018-1046-2.
* Oberg, E.; et al. (2004). Machinery's Handbook (27th ed.). Industrial Press Incorporated.
* Cobb, Harold (September 2007). "The Naming and Numbering of Stainless Steels". Advanced Materials & Processes: 39–44.

* v
* t
* e

SAE International

Organizations|

* Association of Licensed Automobile Manufacturers
* FISITA
* Société des ingénieurs de l'automobile

Standards|

* ARP4754
* ARP4761
* AS9000
* AS9100

* SAE J300
* SAE J306
* SAE J1587
* SAE J1708
* SAE J1772
* SAE J1814
* SAE J1939
* SAE J2452
* SAE J3016
* SAE J3068
* SAE J3105
* SAE J3400

Awards|

* Wright Brothers Medal

People|

* Andrew L. Riker
* Henry Ford

Competitions|

* Baja SAE
* Formula SAE
* SAE Aerodesign
* SAE Supermileage Competition

Related|

* Engineering Societies' Building
* SAE steel grades
* SAE 304
* SAE 316
* SAE 316L
* SAE 440C
* SAE 630
* SAE 904L

*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template